1 New Transparent High-Barrier Film for Advanced Retort Applications Tatsuya Oshita KURARAY CO., LTD ABSTRACT KURARISTER TM, which is henceforth called Hybrid film, is a new transparent high-barrier film for advanced retort applications, and which is a biaxial oriented polyethylene terephthalate (PET) film or a biaxial oriented polyamide (PA) film with a hybrid composite coating on both sides. The hybrid film shows excellent gas barrier properties before and after sterilization that don t depend on humidity, sterilization conditions, or the structure of the laminated film. As the hybrid composite coating layer has excellent scratch resistance and flex resistance, the gas barrier properties are stable during converting, transportation storage, flexing and tension etc. INTRODUCTION Packages for sterilized food have traditionally been metal cans, glass bottles and aluminum foil pouches. Recent developments of pouch structures including transparent plastic barrier films are expected to show growth as replacements for the older materials thanks to their improved properties as Microwave-ability, Metal Detection Capability, and Reduction of incinerated residue [1,2,3]. Against this background, a new hybrid, transparent high-barrier film Hybrid film [4,5] has been developed to meet the requirements of these applications and is already being produced on a commercial scale. Hybrid film shows features, including (a) very high and consistent oxygen barrier before, during and after retort, (b) oxygen barrier performance independent of the retort method, (c) barrier not affected by humidity, elongation (5%), scratching or flexing, (d) high transparency: similar to PET or PA substrates, (e) easy printing without surface pre-treatment, (d) easy handling: no curling, low coefficient of friction. In this paper these features of hybrid film are described based on evaluation results. EXPERIMENTAL The laminated films were prepared with PET based barrier film / ad / PA film / ad / CPP and PA based barrier film / ad / CPP structures. Major properties such as oxygen gas barrier and mechanical properties before / after retort treatment were examined. Detailed experimental materials and test methods are described in Appendix 1. RESULTS AND DISCUSSION 1. Mechanical properties Mechanical properties of both a PET based hybrid film and a PA based hybrid film are summarized in Table 1. Tensile strength at break of both hybrid films was slightly weaker than substrate films. Elongation at break of both hybrid films was the same as substrate films. Tensile modulus of both hybrid films was a little higher than substrate films. The puncture resistance and impact strength of PA based hybrid film was 80 to 90% of PA film, however the values are of a sufficient high level to keep the features of PA based film. Total light transmission of both hybrid films was the same as PET film. In a final comparison, features of the product regarding mechanical properties were almost equal to the substrate films. When PA film is used as the surface layer of a laminated film, mechanical properties of PA film deteriorate during retort by an oxidation reaction. PA based hybrid film is expected to be used in a two layer laminate structure, which is PA based hybrid film // CPP, for retort applications. So, mechanical properties of the two layer laminated film were evaluated before and after retort treatment. For comparison, PA film // CPP was evaluated, too. The results are summarized in table 2. Mechanical properties of PA film // CPP deteriorate, especially impact strength were down to 30% of the before retort levels. On the other hand, in case of PA based hybrid film, mechanical properties after retort were almost equal to those before retort. This good result was attributed to protection of the PA film by the hybrid composition layer.
2 2. Oxygen gas barrier properties. The Oxygen Transmission Rate (OTR) for laminated films before and after retort is listed in Table 3. OTR results of PET based hybrid film were 0.4cc/m 2 /day/atm, and don t depend on retort methods, retort temperature or retort time. In the case of a PA based hybrid film, OTR after retort, under conditions of hot water retort, 120ºC, 30minutes, was 0.7cc/m 2 /day/atm even in the worst case. The relationship between humidity and OTR is shown in Fig.1. OTR is independent of humidity. Concerning PET based inorganic coated film, OTR results were 0.3 to 1.5 cc/m 2 /day/atm with some scatter. These values were dependent on sterilization conditions. 3. Peel strength of laminated film after retort In Table 4 results regarding peel strength of laminated film including hybrid film are summarized. All peel strength results were more than 400g/15mm which is considered sufficient for most retort applications. It was found that peel strength can be improved by choosing a suitable adhesive for hybrid film. 4. Properties related with converting The wetting index of PET based hybrid film and PA based hybrid film was at the same level as each corona treated PET film and corona treated PA film. According to printing test results by customers, both solvent based ink and water based ink could be directly applied to hybrid films by gravure rolls without difficulty. Coefficient of static friction (COF) levels of both PET based hybrid film and PA based hybrid film were similar to PET film. As shown in Figure 2 the COF of hybrid film doesn t depend on humidity and temperature. The COF is low both between hybrid film and hybrid film and between hybrid film and a metal roll. This means easy handling of hybrid film without generating wrinkles during printing and laminating. 5. OTR after abuse test 5% elongation and scratch tests were studied as an indication of abuse resistance. Deterioration of oxygen barrier properties by 5% elongation and gelbo flexing testing was very small as shown in table 6 and Figure 3. Because the matrix phase of the hybrid composition is a polymer with stretchable properties, it was expected that small deformation of the hybrid film would hardly affect gas barrier properties. The hybrid films showed excellent scratch resistance thanks to a strong interaction between polymer and inorganic compounds in the hybrid composition. Furthermore, both side barrier coating of the hybrid film improved reliability of gas barrier properties after abuse tests. In the case of inorganic coated film, scratch resistance and abrasion resistance were not as good due to very thin thickness of the coating layer. CONCLUSIONS 1. Hybrid films consistently show excellent oxygen barrier properties before and after sterilization. The oxygen barrier property does not depend on humidity, or sterilization conditions. 2. Hybrid film has good flex, scratch and 5% elongation resistance thanks to a stretchable polymer matrix phase in the hybrid composition and strong interaction between the polymer and inorganic materials. 3. PA based hybrid film shows good mechanical properties such as impact strength, puncture resistance etc even after sterilization, because the PA substrate is protected by a hybrid composition layer from oxidation reaction during retort. 4. Thanks to similar COF and wetting index properties of the hybrid film with PET film, handling during printing and laminating is easy. ACKOWLEDGMENTS
3 The authors are grateful to the people that support preparing this paper, especially those in EVAL COMPANY of America. REFERENCES 1. Japan Canners Association The Canners Journal, Vol.85, No.8, p (2006) 2. K. Kobayashi Journal of Packaging Science & Technology Japan, Vol.9, No.6, p (2000) 3. T. Katsura PACKPIA, September,p40-45(2000) 4. T. Oshita, Journal of Packaging Science & Technology Japan, Vol.15, No.4, p (2006) 5. T. Oshita, Convertech, No.402, p92-94(2006) Table 1 Mechanical properties of hybrid film Measurement 1) Items Tensile strength at break Elongation at break Units PET based hybrid film PA based hybrid film PET film PA film MD MPa TD MD % TD Tensile modulus MD GPa TD Puncture resistance N Impact strength J Total light transmission % ) Measurement conditions: 23ºC, 50%RH Table 2 Mechanical properties of laminated film PA based hybrid film PA film // CPP Measurement 1) //CPP film Units Items Before After Before After retort retort 2) retort retort 2) Tensile strength MD MPa at break TD Elongation MD % at break TD Tensile modulus MD GPa TD Puncture resistance N Impact strength J ) Measurement condition: 23ºC, 50%RH 2) Retort condition: Hot water retort, 120ºC, 30min Table 3 Oxygen transmission rate (OTR) of laminated film after retort Retort condition (Retort method / Temp. / Time) PET based Hybrid film (1) OTR(cc/m 2 /day/atm) 3) PA based Hybrid film (2) PET based inorganic coated film (1)
4 Before retort Hot water retort / 120ºC / 30min Hot water retort / 120ºC / 60min Hot water retort / 120ºC / 180min Hot water retort / 135ºC / 30min Spray retort / 120ºC / 30min Spray retort / 135ºC / 30min Steam retort / 120ºC / 30min ) Structure of the laminated film: PET based gas barrier film // PA film 15 // CPP 50 2) Structure of the laminated film: PA based gas barrier film // CPP 50 3) OTR measurement condition: 20ºC, 85%RH / 100%RH Table 4 Peel strength of laminated film after retort Retort condition (Retort method / Temp. / Time) Peel strength (g/15mm) 3) PET based Hybrid film 1) PA based Hybrid film 2) Before retort Hot water retort / 120ºC / 30min Hot water retort / 120ºC / 60min Hot water retort / 120ºC / 180min ) Structure of the laminated film: PET based gas barrier film // PA film 15 // CPP 50 2) Structure of the laminated film: PA based gas barrier film // CPP 50 3) Peel strength measurement condition: 23ºC, 50%RH, 3hours later after retort PET based inorganic coated film 1) Table 5 Properties related with converting Measurement 1) Items PET based hybrid film PET film (corona treated) PA based hybrid film PA film (corona treated ) Wetting index >54 >54 >54 50 Coefficient of static friction 1) Measurement conditions:23ºc, 50%RH Table 6 Oxygen transmission rate (OTR) after abuse test OTR(cc/m 2 /day/atm) 1) Abuse test PET based Hybrid film PET based Inorganic coated film Before abuse test % elongation test Scratch test < 1) OTR measurement conditions:20ºc, 85%RH / 85%RH
5 10 OTR (cc/m 2 /day/atm) Relative humidity (%RH) Fig. 1 Relationship between humidity and OTR 1) 1) OTR measurement temperature: 20ºC 5.0 Coefficient of static friction PA based hybrid film PA film Relative humidity (%RH) Fig. 2 Coefficient of static friction vs Relative humidity
6 After retort + Gelbo flexing 50 times After retort + Gelbo flexing 10 times After retort Before retort PET based inorgaic coated film//pa//cpp PET based hybrid film//pa//cpp OTR (cc/m 2 /day/atm) Fig.3 OTR 1) of laminated film after retort and gelbo flexing test 1) OTR measurement condition: 20ºC, 85%RH / 100%RH
7 Appendix 1 Materials (1) KURARISTER TM, which is henceforth called Hybrid film, is a biaxial oriented PET film or a biaxial oriented PA film with hybrid composite coating on both sides. The hybrid composite is composed of a polymer and an inorganic component. (2) Grade of biaxial oriented polyamide (PA) film as a layer of laminated film is EMBLEM ONBC 15 produced by UNITIKA CO., LTD. (3) Grade of cast polypropylene (CPP) film as sealant of laminated film is RXC-18 produced by TOHCELLO CO., LTD. (4) Grade of adhesive (AD) for laminated film is Takelac A-385 and Takenate A-50 produced by MITSUI CHEMICALS POLYURETHANES, INC. (5) Inorganic coated PET film was used for comparison. (6) Structure of laminated film including PET based barrier film is PET based barrier film / ad / PA film / ad / CPP. (7) Structure of laminated film including PA based barrier film is PA based barrier film / ad / CPP. Test methods (1) Oxygen barrier property before sterilization In this test, oxygen transmission rate (OTR) of a barrier film itself or a laminated film including a barrier film is measured under the below condition. Equipment: MOCON10/50, Condition of OTR: 20ºC, 85%RH (Oxygen provided side) / 85%RH (Oxygen detected side) (2) Oxygen barrier property after sterilization A pouch was made from two laminated films including a barrier film and was filled with water. The pouch was sterilized under specific conditions. After sterilization, laminated film samples were cut from the pouch. Water on the surface of the laminated film was removed by paper and OTR was measured under the below conditions. Equipment: MOCON10/50, Condition of OTR: 20ºC, 85%RH (Oxygen provided side) / 100%RH (Oxygen detected side) (3) Tensile strength at break, tensile elongation at break and tensile modulus Equipment: AUTOGRAPH AGS-H (SHIMAZU CORPORATION), Measurement condition: 23ºC, 50%RH, tensile speed in case of tensile strength at break and tensile elongation at break: 200mm/minute, tensile speed in case of tensile modulus: 50mm/minute (4) Puncture resistance Equipment: AUTOGRAPH AGS-H (SHIMAZU CORPORATION), Measurement condition: 23ºC, 50%RH, puncture speed: 50mm/minute, diameter of needle tip: 1mm (5) Impact strength Equipment: Film Impact Tester (Toyo Seiki Seisaku-sho, LTD.), Measurement condition: 23ºC, 50%RH, (6) Total light transmission Equipment: Spectro color meter NF902 (Nippon Denshoku Industries Co., Ltd.), Measurement condition: 23 ºC, 50%RH (7) Wetting index Measurement by using reagent for wet index (Wako Pure Chemical Industries, Ltd.), Measurement condition: 23ºC, 50%RH (8) Coefficient of static friction Equipment: Friction Angle Tester (Toyo Seiki Seisaku-sho, LTD.), Measurement condition: 23ºC, 50%RH, (9) 5% elongation test In 5% elongation test, barrier film is elongated to 5% by using a below equipment. And OTR of samples after elongation is measured. Equipment: handmade equipment with handle, Measurement condition: 23ºC, 50%RH, tensile speed: about 100mm/minute
8 (10) Scratch test In scratch test, back and forth motion of sandpaper on the barrier film by using a below equipment was repeated 5 times. And OTR of samples after scratch test is measured. Equipment: Color Fastness Rubbing Tester (TESTER SANGYO CO., LTD.), Measurement condition: 23ºC, 50%RH, (11) Gelbo flexing test In scratch test, laminated film including barrier film after sterilization is flexed by using below equipment.. And OTR of the laminated film after flexing is measured. Equipment: Gelbo flex tester (Rigaku Kogyo), Measurement condition: 23ºC, 50%RH, number of gelbo flexing 10times, 50times (12) Retort treatment Equipment: Retort treatment machine RCS (HISAKA WORKS, LTD.), Measurement condition: 23ºC, 50%RH,
9 2007 PLACE Conference September St Louis, MO New Transparent High-Barrier Film for Advanced Retort Applications KURARISTER TM Presented by: Tatsuya Oshita Research Manager KURARAY CO., LTD
10 Structure of Hybrid Film Hybrid composite with gas barrier property Both sides coating on a base film PET film or PA film Hybrid composite layer PET or PA film
11 Hybrid Film Flexible Polymer Inorganic Compound High density Stable Strong interaction Restricted polymer molecular movement Gas barrier properties Polymer matrix Resistance to deformation as flexion etc.
12 Features of Hybrid Film Very high and consistent gas barrier before, during and after retort Gas barrier independent of retort conditions Gas barrier not affected by humidity, elongation, scratching or flex Easy printing without surface pre-treatment Easy handling: no curl, very low coefficient of friction (COF)
13 Oxygen Barrier With Varied Retort Conditions Retort Retort method conditions Before retort Hot water 120ºC/30min Hot water 120ºC/180min Hot water 135ºC/30min Spray 135ºC/30min PET based hybrid film (1) OTR (3) (cc/m 2 /day/atm) PA based hybrid film (2) PET based inorganic coated film (1) (1) Sample: Barrier film // PA film15 // CPP film50 (2) Sample: Barrier film // CPP film50 (3) OTR: 20ºC, 85%RH / 100%RH
14 Oxygen Barrier With Varied Retort Methods Before or after Retort Before retort (coated film) Before retort (laminated film) After retort (laminated film) OTR conditions 20ºC 85%RH 20ºC 85/100%RH Hot water (1) OTR (cc/m 2 /day/atm) Spray (1) Steam (1) (1) Retort conditions: 120ºC, 30min.
15 OTR vs. Relative Humidity OTR (cc/m 2 /day/atm) Relative humidity (%RH)
16 Printability Solvent based ink Water based ink Hybrid film / Solvent based ink / Ad / PA film / Ad / CPP Wetting index(dyne/cm) PET based hybrid film PET film (no corona treatment) (corona treated) >54 >54
17 Coefficient of Static Friction Film sample Weight 92g Θ tanθ PET based hybrid film 0.45 Coefficient of static friction (1) PA based hybrid film 0.47 PET film 0.58 (1)Coefficient of static friction: 23ºC, 50%RH PA film 1.11
18 Humidity-Dependence of Coefficient of Static Friction Coefficient of static friction (1) PA based hybrid film PA film Relative humidity (%RH) (1) Temperature: 23ºC
19 Abuse in Production Process Scratching/expanding Converting Folding/sealing Pouch making Expanding/sealing Filling Expanding/shrink Retort Hitting Transportation Market
20 Evaluation method Scratch Resistance OTR after scratching 5 times on barrier layer Sand paper(#2000) Film for scratch test Weight 100g Arm Adhesive tape Containerboard for fixing the film Back-and-forth motion of the containerboard with the film
21 OTR after Scratch Test OTR (2) (cc/m 2 /day/atm) Scratch (1) times 0 time 5 times PET based hybrid film PET based Inorganic coated film 0.3 >40 (1) Scratch Conditions: 23ºC, 50%RH (2) OTR: 20ºC, 85%RH / 85%RH
22 Stress-Strain Strain Hysteresis Curve Plastic deformation in more than 3% strain Stress (kgf) Strain (%)
23 OTR after Elongation Elongation (1) Ratio OTR (2) (cc/m 2 /day/atm) PET based hybrid film PA based hybrid film 0% 5% (1) Elongation: 23ºC, 50%RH, 100mm/min (2) OTR: 20ºC, 85%RH / 85%RH Handle for elongation Film
24 OTR after Folding & Retort Hot water retort Pouch 120ºC 30min. Laminated film Folding OTR (1) (cc/m 2 /day/atm) After folding & retort 0.4 (1) OTR: 20 o C-85%RH/100%RH After retort 0.4
25 OTR after Gelbo Flex Retort Gelbo flex OTR Retort + Gelbo 50times Retort + Gelbo 10times Retort Before retort PET based inorgaic coated film PA based hybrid film PET based hybrid film OTR (cc/m 2 /day/atm)
26 Reliability of Gas Barrier - Lidding film - Teat sample Damage by heat seal Lidding film Barrier film//pa film//cpp film Gel Gel + O 2 Blue gel Damage by shrinkage
27 Before retort Lidding Film After retort A B C A B C A B C EVOH film PET based Hybrid film PET based Inorganic coated film
28 Deterioration of PA During Retort Deterioration by oxygen attacks during retort Protection by hybrid gas barrier layer O 2 O 2 O 2 O 2 O 2 O 2 Barrier CPP Hybrid film Conventional barrier film PA Ad
29 Mechanical Properties of Measurement items Tensile modulus Impact strength Laminated Film Tensile strength MD MPa at break TD Elongation MD % at break TD MD TD Puncture resistance Units GPa N J PA based hybrid film//cpp film Before retort After retort PA film//cpp Before retort After retort
30 Conclusions Excellent and consistent gas barrier properties Gas barrier independent of retort conditions Gas barrier not affected by humidity, elongation, scratching nor flexing Easy printing without surface pre-treatment Easy handling: no curl, very low coefficient of friction
31 Thank You PRESENTED BY Tatsuya Oshita Research Manager KURARAY CO., LTD Please remember to turn in your evaluation sheet...